Microstructure and mechanical properties of electron beam ...wrap. and mechanical...2 Keywords:...
Embed Size (px)
Transcript of Microstructure and mechanical properties of electron beam ...wrap. and mechanical...2 Keywords:...
Original citation: Dinda, Soumitra Kumar, Basiruddin Sk, Md., Roy, Gour Gopal and Srirangam, Prakash. (2016) Microstructure and mechanical properties of electron beam welded dissimilar steel to Fe-Al alloy joints. Materials Science and Engineering: A . doi: 10.1016/j.msea.2016.09.050 Permanent WRAP URL: http://wrap.warwick.ac.uk/81655 Copyright and reuse: The Warwick Research Archive Portal (WRAP) makes this work by researchers of the University of Warwick available open access under the following conditions. Copyright and all moral rights to the version of the paper presented here belong to the individual author(s) and/or other copyright owners. To the extent reasonable and practicable the material made available in WRAP has been checked for eligibility before being made available. Copies of full items can be used for personal research or study, educational, or not-for-profit purposes without prior permission or charge. Provided that the authors, title and full bibliographic details are credited, a hyperlink and/or URL is given for the original metadata page and the content is not changed in any way. Publishers statement: 2016, Elsevier. Licensed under the Creative Commons Attribution-NonCommercial-NoDerivatives 4.0 International http://creativecommons.org/licenses/by-nc-nd/4.0/
A note on versions: The version presented here may differ from the published version or, version of record, if you wish to cite this item you are advised to consult the publishers version. Please see the permanent WRAP url above for details on accessing the published version and note that access may require a subscription. For more information, please contact the WRAP Team at: firstname.lastname@example.org
Microstructure and mechanical properties of electron beam welded
dissimilar steel to Fe-Al alloy joints
Soumitra Kumar Dindaa, Md. Basiruddin Sk
a, Gour Gopal Roy
a, Prakash Srirangam
aDepartment of Metallurgical and Materials Engineering, Indian Institute of Technology, Kharagpur, India.
bWarwick Manufacturing Group (WMG), University of Warwick, Coventry, CV4 7AL, UK
*Corresponding author: email@example.com
Electron beam welding (EBW) technique was used to perform dissimilar joining of plain
carbon steel to Fe-7%Al alloy under three different weld conditions such as with beam
oscillation, without beam oscillation and at higher welding speed. The effect of weld
parameters on the microstructure and mechanical properties of dissimilar joints was studied
using optical microscopy, SEM, EBSD, hardness, tensile and erichsen cup tests.
Microstructure results show that the application of beam oscillation resulted in uniform and
homogeneous microstructure compared to without beam oscillations and higher welding
speed. Further, it was observed that weld microstructure changes from equiaxed to columnar
grains depending on the weld speed. High weld speed results in columnar grain structure in
the weld joint. Erichsen cup test results show that the application of beam oscillation results
in excellent formability as compared to high weld speed. Tensile test results show no
significant difference in strength properties in all three weld conditions, but the ductility was
found to be highest for joints obtained with the application of weld beam oscillation as
compared to without beam oscillation and high weld speed. This study shows that the
application of beam oscillations plays an important role in improving the weld quality and
performance of EBW dissimilar steel to Fe-Al joints.
Keywords: Electron beam welding, steel, Fe-Al alloy, microstructure, EBSD, mechanical
properties, erichsen cup test, fractography.
The demand for the development of light weight materials has been increasing in automotive
and aerospace industries to meet the challenges of fuel saving and greenhouse gas emissions.
Hence, the transportation industry is in search of alternatives to meet these challenges and
light weighting is the promising strategy in the field of automotive, nuclear, thermal power,
chemical and petrochemical industries to enhance fuel efficiency and to reduce greenhouse
gas emissions [1, 2, 3]. It is known that a reduction of 10% of total weight of the vehicle
improves the fuel efficiency of passenger cars by 6-8% . One method of reducing the
weight of steel alloys is to add higher amounts of aluminium to steel. Addition of 7-8%
aluminium reduces the density of steel by about 17% . However, forming and welding of
low density steels to other car body parts made of different alloy materials especially with
steel parts is challenging due to the different physical, mechanical and metallurgical
properties of dissimilar metals . Arc welding processes which operates at very high heat
input in comparison to EBW, favours the formation of different brittle Fe-Al intermetallics at
the weld interface which deteriorates mechanical properties of weld dissimilar joints .
EBW is one of the best fusion welding processes which provides good mechanical and
metallurgical properties in comparison to other welding processes such as friction stir
welding, explosive welding, ultrasonic welding, arc welding, laser beam welding etc. [8, 9].
EBW has advantages such as high power density, low heat input, high penetration, low
distortion, high depth to width ratio, narrow HAZ, less contamination from environments,
and minimum amount of defects . Due to low heat input, very high power density and
zero environmental contamination in EBW, the chances of defect formation is less in EBW
dissimilar joints .
Optimisation of weld parameters is very important in welding process to achieve a sound
weld quality with uniform microstructure and excellent mechanical properties of dissimilar
weld joints. Metallurgical and mechanical property characterization of dissimilar welded
joints is therefore essential to understand the influence of weld parameters on structure
property relationships of joints. Saresh et al. studied EB-welding of thick Ti-6Al-4V alloy
joints and found that the weld quality was improved with double sided welding as compared
to single sided welding . Babu et al. studied the effect of beam oscillations on the weld
microstructure and mechanical properties of Ti-6Al-4V alloy system. They observed that the
application of beam oscillations resulted in lower hardness and higher ductility in the weld
region compared to without beam oscillation condition . Sierra et al. studied the effect of
weld parameters on mechanical properties of laser welded dissimilar joints of low carbon
steel to aluminium alloy . Bandhyopadhyay et al. studied the formability of laser welded
high strength steel sheet joints by erichsen cupping test and validated the results with finite
element modelling . Kar et al. studied the effect of beam oscillation on the mechanical
properties of EB-welded Cu-SS joint and reported that toughness of the joint increases
significantly due to the application of weld beam oscillations . Tomashchuk et al. studied
the effect of weld parameters on the microstructures and mechanical properties of EB-welded
titanium alloys to AISI 316L austenitic SS . However, from literature review and past
research studies, it was clear that the methods to improve microstructures and mechanical
properties of EBW welded steel to Fe-Al alloy dissimilar joints has not been thoroughly
studied in the past. In the present study, we aimed at understanding the effect of weld
parameters on microstructure and mechanical properties of dissimilar steel to Fe-7% Al alloy
joints by EBW. Microstructural and mechanical properties characterisations were performed
using optical microscopy, SEM, EBSD, hardness, tensile testing, and erichsen cup tests.
Plain carbon steel and Fe-Al alloys were used as base materials for EBW of dissimilar
joining. Fe-Al alloy plates were supplied by Tata Steel R&D Corporation, Swindon, UK and
steels were commercially purchased from N. Maity & Co., Kharagpur, India. Chemical
analysis of base materials used in joining were analysed by X-ray spectroscopy analysis.
Table 1 represents the chemical composition of base materials used in this study.
Table 1. Chemical composition of base materials in weight %.
Base Material C Al Mn Si P S Nb Ti Fe
Fe-Al alloy 0.0044 6.94 0.20 - - - 0.01 0.01 Bal
Plain C-Steel 0.3 0.08 0.92 0.23 0.02 0.02 - - Bal
In order to perform welding, base materials were cut into 100 mm (L) x100 mm (W)
dimensions having 1mm thickness of both side materials using diamond wheel cutter with
water cooling system, mechanically polished using 320 grit emery papers and subsequently
cleaned with acetone. Fig. 1 shows the schematic of EBW process with the application of
beam oscillation. Beam oscillation was applied to modify the weld quality. Beam oscillation
employs electromagnetic fields to alter the direction of electron beam as shown in Fig. 1b.
Electron beam oscillati